#------------------------------------------------------------------------------
#$Date: 2024-07-05 19:44:31 +0300 (Fri, 05 Jul 2024) $
#$Revision: 293117 $
#$URL: file:///home/coder/svn-repositories/cod/cif/7/71/58/7715834.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7715834
loop_
_publ_author_name
'Handzlik, Gabriela'
'Dziubek, Kamil F.'
'Hanfland, Michael'
'Pinkowicz, Dawid'
_publ_section_title
;
 Simultaneous manipulation of iron(II) spin crossover and LIESST behaviour
 using pressure, temperature and light.
;
_journal_issue                   18
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              7677
_journal_page_last               7681
_journal_paper_doi               10.1039/d4dt00509k
_journal_volume                  53
_journal_year                    2024
_chemical_formula_moiety         'C32 H32 Fe2 N24 Nb, 4(H2 O)'
_chemical_formula_sum            'C32 H40 Fe2 N24 Nb O4'
_chemical_formula_weight         1029.49
_chemical_name_systematic
'catena-[tetrakis(m2-Cyano)-octakis(1H-pyrazole-N2)-tetracyano-di-iron(ii)-niobium(iv) tetrahydrate]'
_chemical_properties_physical    Air-sensitive
_space_group_crystal_system      tetragonal
_space_group_IT_number           88
_space_group_name_Hall           '-I 4ad'
_space_group_name_H-M_alt        'I 41/a :2'
_atom_sites_solution_hydrogens   mixed
_atom_sites_solution_primary     dual
_audit_creation_date             2024-01-17
_audit_creation_method
;
Olex2 1.5
(compiled 2023.08.24 svn.re1ec1418 for OlexSys, GUI svn.r6817)
;
_audit_update_record
;
2024-03-15 deposited with the CCDC.	2024-04-09 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   21.4722(3)
_cell_length_b                   21.4722(3)
_cell_length_c                   9.4522(8)
_cell_measurement_reflns_used    1317
_cell_measurement_temperature    5.00
_cell_measurement_theta_max      19.8630
_cell_measurement_theta_min      1.7420
_cell_volume                     4358.0(4)
_computing_cell_refinement       'CrysAlisPro 1.171.41.119a (Rigaku OD, 2021)'
_computing_data_collection       'CrysAlisPro 1.171.41.119a (Rigaku OD, 2021)'
_computing_data_reduction        'CrysAlisPro 1.171.41.119a (Rigaku OD, 2021)'
_computing_molecular_graphics    'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_structure_refinement  'SHELXL 2019/2 (Sheldrick, 2015)'
_computing_structure_solution    'SHELXT 2018/2 (Sheldrick, 2018)'
_diffrn_ambient_pressure         280000
_diffrn_ambient_temperature      5.00
_diffrn_detector                 'Hybrid Pixel Array Detector'
_diffrn_detector_area_resol_mean 13.3333
_diffrn_measured_fraction_theta_full 0.660
_diffrn_measured_fraction_theta_max 0.386
_diffrn_measurement_details
;
List of Runs (angles in degrees, time in seconds):

  # Type    Start    End  Width  tₑₓₚ   ω     θ     κ     φ   Frames
#--------------------------------------------------------------------------
  1  ω    -32.00  32.00   0.50    0.20    --    0.00   0.00   0.00  128
;
_diffrn_measurement_device       'abstract diffractometer'
_diffrn_measurement_device_type
'esperanto-CrysAlisPro-abstract goniometer imported esperanto images'
_diffrn_measurement_method       'ω scans'
_diffrn_orient_matrix_type
'CrysAlisPro convention (1999,Acta A55,543-557)'
_diffrn_orient_matrix_UB_11      -0.0003879000
_diffrn_orient_matrix_UB_12      -0.0080441000
_diffrn_orient_matrix_UB_13      -0.0393195000
_diffrn_orient_matrix_UB_21      0.0023288000
_diffrn_orient_matrix_UB_22      -0.0172071000
_diffrn_orient_matrix_UB_23      0.0180495000
_diffrn_orient_matrix_UB_31      -0.0189611000
_diffrn_orient_matrix_UB_32      -0.0019560000
_diffrn_orient_matrix_UB_33      0.0030361000
_diffrn_radiation_monochromator  synchrotron
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           synchrotron
_diffrn_radiation_wavelength     0.41008
_diffrn_reflns_av_R_equivalents  0.0462
_diffrn_reflns_av_unetI/netI     0.0619
_diffrn_reflns_Laue_measured_fraction_full 0.660
_diffrn_reflns_Laue_measured_fraction_max 0.386
_diffrn_reflns_limit_h_max       28
_diffrn_reflns_limit_h_min       -27
_diffrn_reflns_limit_k_max       27
_diffrn_reflns_limit_k_min       -28
_diffrn_reflns_limit_l_max       8
_diffrn_reflns_limit_l_min       -8
_diffrn_reflns_number            4513
_diffrn_reflns_point_group_measured_fraction_full 0.660
_diffrn_reflns_point_group_measured_fraction_max 0.386
_diffrn_reflns_theta_full        14.244
_diffrn_reflns_theta_max         19.966
_diffrn_reflns_theta_min         1.744
_diffrn_source                   'ESRF ID15B'
_exptl_absorpt_coefficient_mu    0.544
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.93825
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlisPro 1.171.41.119a (Rigaku Oxford Diffraction, 2021)
Empirical absorption correction using spherical harmonics,
implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            violet
_exptl_crystal_density_diffrn    1.569
_exptl_crystal_description       block
_exptl_crystal_F_000             2100
_exptl_crystal_preparation       'Magnetic properties'
_exptl_crystal_recrystallization_method 'Re-crystallisation from solvent: water'
_exptl_crystal_size_max          0.1
_exptl_crystal_size_mid          0.1
_exptl_crystal_size_min          0.03
_refine_diff_density_max         0.361
_refine_diff_density_min         -0.332
_refine_diff_density_rms         0.074
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.048
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     152
_refine_ls_number_reflns         2039
_refine_ls_number_restraints     3
_refine_ls_restrained_S_all      1.051
_refine_ls_R_factor_all          0.0418
_refine_ls_R_factor_gt           0.0351
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0386P)²] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0892
_refine_ls_wR_factor_ref         0.0930
_reflns_Friedel_coverage         0.000
_reflns_number_gt                1767
_reflns_number_total             2039
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            d4dt00509k2.cif
_cod_data_source_block           fenb_0014
_cod_depositor_comments
'Adding full bibliography for 7715833--7715849.cif.'
_cod_original_sg_symbol_H-M      'I 41/a'
_cod_database_code               7715834
_shelx_shelxl_version_number     2019/2
_chemical_oxdiff_formula         'C11 H10 N O'
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_olex2_refinement_description
;
1. Fixed Uiso
 At 1.2 times of:
  All C(H) groups, All N(H) groups
2. Restrained distances
 O1-H1
 0.95 with sigma of 0.02
 O1-H2
 0.95 with sigma of 0.02
 H1-H2
 1.5 with sigma of 0.04
3.a Aromatic/amide H refined with riding coordinates:
 N4(H3), N6(H7), C6(H10), C5(H4), C8(H8), C7(H9), C3(H6), C4(H5)
;
_olex2_submission_special_instructions 'No special instructions were received'
_oxdiff_diffrn_reflns_filtered   274
_oxdiff_exptl_absorpt_empirical_details
;
Empirical correction (ABSPACK) includes:
- Absorption correction using spherical harmonics
- Frame scaling
- Detector area scaling
;
_oxdiff_exptl_absorpt_empirical_full_max 1.199
_oxdiff_exptl_absorpt_empirical_full_min 0.847
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x+1/2, -y, z+1/2'
'-y+3/4, x+1/4, z+1/4'
'y+3/4, -x+3/4, z+3/4'
'x+1/2, y+1/2, z+1/2'
'-x+1, -y+1/2, z+1'
'-y+5/4, x+3/4, z+3/4'
'y+5/4, -x+5/4, z+5/4'
'-x, -y, -z'
'x-1/2, y, -z-1/2'
'y-3/4, -x-1/4, -z-1/4'
'-y-3/4, x-3/4, -z-3/4'
'-x+1/2, -y+1/2, -z+1/2'
'x, y+1/2, -z'
'y-1/4, -x+1/4, -z+1/4'
'-y-1/4, x-1/4, -z-1/4'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Nb1 Nb 0.500000 0.750000 0.625000 0.01272(17) Uani 1 4 d S T P . .
Fe1 Fe 0.500000 0.500000 0.500000 0.0148(2) Uani 1 2 d S . P . .
O1 O 0.44020(8) 0.63426(8) 0.1952(4) 0.0203(8) Uani 1 1 d D . . . .
N2 N 0.48329(9) 0.59903(9) 0.5200(4) 0.0183(8) Uani 1 1 d . . . . .
N4 N 0.45276(9) 0.53567(9) 0.7973(4) 0.0189(9) Uani 1 1 d . . . . .
H3 H 0.466019 0.573539 0.778347 0.023 Uiso 1 1 calc R U . . .
N5 N 0.41472(8) 0.48314(8) 0.3865(3) 0.0193(9) Uani 1 1 d . . . . .
N3 N 0.45470(9) 0.48789(8) 0.7035(4) 0.0184(8) Uani 1 1 d . . . . .
N1 N 0.51429(9) 0.83938(9) 0.9198(4) 0.0212(9) Uani 1 1 d . . . . .
N6 N 0.38989(9) 0.52256(9) 0.2908(4) 0.0184(9) Uani 1 1 d . . . . .
H7 H 0.407460 0.557529 0.263210 0.022 Uiso 1 1 calc R U . . .
C2 C 0.48685(10) 0.65037(10) 0.5552(4) 0.0167(9) Uani 1 1 d . . . . .
C6 C 0.37410(11) 0.43611(10) 0.3979(4) 0.0201(10) Uani 1 1 d . . . . .
H10 H 0.379573 0.400962 0.457675 0.024 Uiso 1 1 calc R U . . .
C5 C 0.42846(11) 0.51878(11) 0.9214(4) 0.0205(10) Uani 1 1 d . . . . .
H4 H 0.422602 0.544647 1.001861 0.025 Uiso 1 1 calc R U . . .
C8 C 0.33455(10) 0.50137(11) 0.2430(4) 0.0216(11) Uani 1 1 d . . . . .
H8 H 0.308528 0.521199 0.175303 0.026 Uiso 1 1 calc R U . . .
C1 C 0.50943(10) 0.80972(10) 0.8196(4) 0.0168(10) Uani 1 1 d . . . . .
C7 C 0.32277(11) 0.44556(11) 0.3105(4) 0.0219(10) Uani 1 1 d . . . . .
H9 H 0.287420 0.419383 0.299631 0.026 Uiso 1 1 calc R U . . .
C3 C 0.43064(10) 0.43976(11) 0.7752(4) 0.0199(10) Uani 1 1 d . . . . .
H6 H 0.425929 0.399019 0.737552 0.024 Uiso 1 1 calc R U . . .
C4 C 0.41355(11) 0.45665(11) 0.9104(4) 0.0240(11) Uani 1 1 d . . . . .
H5 H 0.395364 0.430894 0.980916 0.029 Uiso 1 1 calc R U . . .
H1 H 0.4540(13) 0.6413(13) 0.103(2) 0.020(9) Uiso 1 1 d D . . . .
H2 H 0.4404(18) 0.6660(15) 0.254(4) 0.067(14) Uiso 1 1 d D . . . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C -0.0011 0.0005 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Fe Fe 0.1482 0.3017 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N -0.0016 0.0010 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Nb Nb -0.0343 1.6958 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O -0.0014 0.0018 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
C2 Nb1 C2 94.90(6) . 12_767 ?
C2 Nb1 C2 94.90(6) 6_564 15_566 ?
C2 Nb1 C2 146.0(2) 12_767 15_566 ?
C2 Nb1 C2 146.0(2) . 6_564 ?
C2 Nb1 C2 94.91(6) . 15_566 ?
C2 Nb1 C2 94.90(6) 12_767 6_564 ?
C1 Nb1 C2 142.19(12) . . ?
C1 Nb1 C2 71.80(12) . 6_564 ?
C1 Nb1 C2 77.00(10) . 15_566 ?
C1 Nb1 C2 77.00(10) 12_767 . ?
C1 Nb1 C2 77.00(10) 15_566 6_564 ?
C1 Nb1 C2 75.36(10) 15_566 . ?
C1 Nb1 C2 75.36(10) 6_564 15_566 ?
C1 Nb1 C2 71.80(12) 6_564 . ?
C1 Nb1 C2 75.36(10) 12_767 6_564 ?
C1 Nb1 C2 75.36(10) . 12_767 ?
C1 Nb1 C2 142.20(12) 6_564 6_564 ?
C1 Nb1 C2 142.20(13) 12_767 12_767 ?
C1 Nb1 C2 71.80(13) 12_767 15_566 ?
C1 Nb1 C2 71.80(13) 15_566 12_767 ?
C1 Nb1 C2 77.00(10) 6_564 12_767 ?
C1 Nb1 C2 142.20(13) 15_566 15_566 ?
C1 Nb1 C1 131.88(10) . 15_566 ?
C1 Nb1 C1 131.88(10) . 12_767 ?
C1 Nb1 C1 131.88(10) 12_767 6_564 ?
C1 Nb1 C1 131.88(10) 15_566 6_564 ?
C1 Nb1 C1 70.42(15) 12_767 15_566 ?
C1 Nb1 C1 70.42(15) . 6_564 ?
N2 Fe1 N2 180.00(10) 9_666 . ?
N2 Fe1 N3 88.06(10) . . ?
N2 Fe1 N3 91.94(10) . 9_666 ?
N2 Fe1 N3 91.94(10) 9_666 . ?
N2 Fe1 N3 88.06(10) 9_666 9_666 ?
N5 Fe1 N2 86.12(8) 9_666 . ?
N5 Fe1 N2 93.88(8) 9_666 9_666 ?
N5 Fe1 N2 86.12(8) . 9_666 ?
N5 Fe1 N2 93.88(8) . . ?
N5 Fe1 N5 180.0 . 9_666 ?
N5 Fe1 N3 87.69(10) 9_666 . ?
N5 Fe1 N3 92.31(10) . . ?
N5 Fe1 N3 92.31(10) 9_666 9_666 ?
N5 Fe1 N3 87.69(10) . 9_666 ?
N3 Fe1 N3 180.0 . 9_666 ?
H1 O1 H2 118(3) . . ?
C2 N2 Fe1 162.3(2) . . ?
N3 N4 H3 123.8 . . ?
C5 N4 H3 123.8 . . ?
C5 N4 N3 112.4(2) . . ?
N6 N5 Fe1 124.39(14) . . ?
C6 N5 Fe1 129.9(2) . . ?
C6 N5 N6 105.7(2) . . ?
N4 N3 Fe1 120.14(17) . . ?
C3 N3 Fe1 135.5(2) . . ?
C3 N3 N4 103.9(3) . . ?
N5 N6 H7 124.4 . . ?
N5 N6 C8 111.2(2) . . ?
C8 N6 H7 124.4 . . ?
N2 C2 Nb1 176.59(18) . . ?
N5 C6 H10 124.5 . . ?
N5 C6 C7 111.0(3) . . ?
C7 C6 H10 124.5 . . ?
N4 C5 H4 126.6 . . ?
N4 C5 C4 106.7(3) . . ?
C4 C5 H4 126.6 . . ?
N6 C8 H8 126.3 . . ?
N6 C8 C7 107.4(3) . . ?
C7 C8 H8 126.3 . . ?
N1 C1 Nb1 179.0(3) . . ?
C6 C7 H9 127.6 . . ?
C8 C7 C6 104.8(2) . . ?
C8 C7 H9 127.6 . . ?
N3 C3 H6 124.2 . . ?
N3 C3 C4 111.7(2) . . ?
C4 C3 H6 124.2 . . ?
C5 C4 C3 105.3(3) . . ?
C5 C4 H5 127.4 . . ?
C3 C4 H5 127.4 . . ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Nb1 C2 2.256(2) . ?
Nb1 C2 2.257(2) 15_566 ?
Nb1 C2 2.257(2) 6_564 ?
Nb1 C2 2.257(2) 12_767 ?
Nb1 C1 2.252(4) . ?
Nb1 C1 2.252(4) 6_564 ?
Nb1 C1 2.252(4) 12_767 ?
Nb1 C1 2.252(4) 15_566 ?
Fe1 N2 2.1647(19) . ?
Fe1 N2 2.1647(19) 9_666 ?
Fe1 N5 2.153(2) . ?
Fe1 N5 2.153(2) 9_666 ?
Fe1 N3 2.171(3) . ?
Fe1 N3 2.171(3) 9_666 ?
O1 H1 0.932(18) . ?
O1 H2 0.880(18) . ?
N2 C2 1.154(3) . ?
N4 H3 0.8800 . ?
N4 N3 1.356(4) . ?
N4 C5 1.335(5) . ?
N5 N6 1.348(4) . ?
N5 C6 1.339(3) . ?
N3 C3 1.340(4) . ?
N1 C1 1.146(5) . ?
N6 H7 0.8800 . ?
N6 C8 1.350(3) . ?
C6 H10 0.9500 . ?
C6 C7 1.393(4) . ?
C5 H4 0.9500 . ?
C5 C4 1.376(3) . ?
C8 H8 0.9500 . ?
C8 C7 1.381(4) . ?
C7 H9 0.9500 . ?
C3 H6 0.9500 . ?
C3 C4 1.378(5) . ?
C4 H5 0.9500 . ?
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
Fe1 N5 N6 C8 -176.5(2) . . . . ?
Fe1 N5 C6 C7 176.0(2) . . . . ?
Fe1 N3 C3 C4 172.8(2) . . . . ?
N4 N3 C3 C4 0.4(3) . . . . ?
N4 C5 C4 C3 0.1(3) . . . . ?
N5 N6 C8 C7 0.0(4) . . . . ?
N5 C6 C7 C8 0.6(4) . . . . ?
N3 N4 C5 C4 0.1(3) . . . . ?
N3 C3 C4 C5 -0.3(3) . . . . ?
N6 N5 C6 C7 -0.6(4) . . . . ?
N6 C8 C7 C6 -0.3(4) . . . . ?
C6 N5 N6 C8 0.4(4) . . . . ?
C5 N4 N3 Fe1 -174.19(18) . . . . ?
C5 N4 N3 C3 -0.3(3) . . . . ?
